Gas phase coating is carried out at higher temperatures, about 1080 °C. The coating material is usually loaded onto trays without physical contact with the parts to be coated. The coating mixture contains active coating material and activator, but usually not thermal ballast. As in the pack cementation process, gaseous aluminium chloride (or fluoride) is transferred to the surface of the part. However, in this case the diffusion is outwards. This kind of coating also requires diffusion heat treatment.